# Electronic Supplementary Material (ESI) for Inorganic Chemistry Frontiers.
# This journal is © the Partner Organisations 2021

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_database_code_depnum_ccdc_archive 'CCDC 2090160'
loop_
_audit_author_name
_audit_author_address
shinian
;Fuzhou university
China
;
_audit_update_record             
;
2021-08-20 deposited with the CCDC.	2021-10-06 downloaded from the CCDC.
;
_audit_creation_date             2021-08-17
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2018/1
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Co K Na2 Nb18 O66 Si, 13(O)'
_chemical_formula_sum            'Co H0 K Na2 Nb18 O79 Si'
_chemical_formula_weight         3108.48
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Nb Nb -2.0727 0.6215 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/c 1'
_space_group_name_Hall           '-P 2ybc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   13.0869(11)
_cell_length_b                   18.0361(14)
_cell_length_c                   35.448(3)
_cell_angle_alpha                90
_cell_angle_beta                 98.134(2)
_cell_angle_gamma                90
_cell_volume                     8282.8(12)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    9794
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      25.10
_cell_measurement_theta_min      2.45
_shelx_estimated_absorpt_T_max   0.769
_shelx_estimated_absorpt_T_min   0.732
_exptl_absorpt_coefficient_mu    2.768
_exptl_absorpt_correction_T_max  0.7452
_exptl_absorpt_correction_T_min  0.5880
_exptl_absorpt_correction_type   none
_exptl_absorpt_process_details   
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.0745 before and 0.0507 after correction.
The Ratio of minimum to maximum transmission is 0.7890.
The λ/2 correction factor is Not present.
;
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            Pink
_exptl_crystal_density_diffrn    2.493
_exptl_crystal_density_meas      .
_exptl_crystal_density_method    ?
_exptl_crystal_description       Block
_exptl_crystal_F_000             5808
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.11
_exptl_crystal_size_min          0.1
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0348
_diffrn_reflns_av_unetI/netI     0.0379
_diffrn_reflns_Laue_measured_fraction_full 0.955
_diffrn_reflns_Laue_measured_fraction_max 0.955
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       40
_diffrn_reflns_limit_l_min       -42
_diffrn_reflns_number            46071
_diffrn_reflns_point_group_measured_fraction_full 0.955
_diffrn_reflns_point_group_measured_fraction_max 0.955
_diffrn_reflns_theta_full        25.108
_diffrn_reflns_theta_max         25.108
_diffrn_reflns_theta_min         1.935
_diffrn_ambient_temperature      296.15
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.955
_diffrn_measured_fraction_theta_max 0.955
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                12622
_reflns_number_total             14105
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       'SAINT V8.38A (?, 2016)'
_computing_data_collection       ?
_computing_data_reduction        'SAINT V8.38A (?, 2016)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'XS (Sheldrick, 2008)'
_refine_diff_density_max         4.209
_refine_diff_density_min         -2.630
_refine_diff_density_rms         0.278
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.063
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     889
_refine_ls_number_reflns         14105
_refine_ls_number_restraints     18
_refine_ls_R_factor_all          0.0842
_refine_ls_R_factor_gt           0.0775
_refine_ls_restrained_S_all      1.067
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0685P)²+316.2612P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1779
_refine_ls_wR_factor_ref         0.1819
_refine_special_details          ?
_olex2_refinement_description    
;
1. Uiso/Uaniso restraints and constraints
Uanis(O52) \\sim Ueq, Uanis(O72) \\sim Ueq, Uanis(O76) \\sim Ueq, : with sigma
of 0.005 and sigma for terminal atoms of 0.01
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Nb1 Nb 0.54092(8) 0.10708(6) 0.11330(3) 0.0232(3) Uani 1 1 d . . . . .
Nb2 Nb 0.37263(9) 0.26033(6) 0.08058(3) 0.0197(2) Uani 1 1 d . . . . .
Nb3 Nb 0.18631(9) 0.33937(6) 0.02118(3) 0.0197(2) Uani 1 1 d . . . . .
Nb4 Nb 0.27891(8) -0.10449(6) 0.18101(3) 0.0179(2) Uani 1 1 d . . . . .
Nb5 Nb 0.09499(8) -0.00565(6) 0.12470(3) 0.0184(2) Uani 1 1 d . . . . .
Nb6 Nb 0.33687(8) -0.03031(6) 0.09855(3) 0.0167(2) Uani 1 1 d . . . . .
Nb7 Nb 0.20249(9) 0.06682(6) 0.22218(3) 0.0220(3) Uani 1 1 d . . . . .
Nb8 Nb 0.46812(9) 0.04092(6) 0.19437(3) 0.0213(3) Uani 1 1 d . . . . .
Nb9 Nb 0.38894(10) 0.44015(6) 0.06379(3) 0.0286(3) Uani 1 1 d . . . . .
Nb10 Nb 0.12977(9) 0.28738(6) 0.10633(3) 0.0197(2) Uani 1 1 d . . . . .
Nb11 Nb 0.01410(9) 0.16173(7) 0.16827(3) 0.0244(3) Uani 1 1 d . . . . .
Nb12 Nb 0.15263(10) 0.46648(6) 0.08937(3) 0.0269(3) Uani 1 1 d . . . . .
Nb13 Nb 0.48942(10) 0.22556(6) 0.18262(3) 0.0252(3) Uani 1 1 d . . . . .
Nb14 Nb 0.33597(10) 0.38366(6) 0.15002(3) 0.0269(3) Uani 1 1 d . . . . .
Nb15 Nb 0.07200(9) -0.18695(6) 0.13188(3) 0.0251(3) Uani 1 1 d . . . . .
Nb16 Nb 0.13004(9) -0.10924(6) 0.05060(3) 0.0210(3) Uani 1 1 d . . . . .
Nb17 Nb 0.30870(9) -0.21191(6) 0.10589(3) 0.0223(3) Uani 1 1 d . . . . .
Nb18 Nb 0.22414(10) 0.25192(6) 0.21049(3) 0.0268(3) Uani 1 1 d . . . . .
Co1 Co 0.52037(19) 0.39436(13) 0.23752(7) 0.0472(6) Uani 1 1 d . . . . .
Si1 Si 0.2694(2) 0.13399(17) 0.13501(8) 0.0152(6) Uani 1 1 d . . . . .
K1 K -0.0864(2) 0.32205(16) -0.04933(8) 0.0320(7) Uani 1 1 d . . . . .
Na1 Na -0.2222(4) 0.3706(3) 0.03124(14) 0.0285(11) Uani 1 1 d . . . . .
Na2 Na 0.7613(5) 0.4981(3) 0.10859(16) 0.0374(13) Uani 1 1 d . . . . .
O1 O 0.3933(6) 0.1282(4) 0.1492(2) 0.0189(17) Uani 1 1 d . . . . .
O2 O 0.2504(6) -0.0385(4) 0.0513(2) 0.0187(17) Uani 1 1 d . . . . .
O3 O 0.3958(8) 0.4034(4) 0.1968(2) 0.028(2) Uani 1 1 d . . . . .
O4 O 0.0739(8) -0.1136(5) 0.0023(2) 0.030(2) Uani 1 1 d . . . . .
O5 O 0.3042(7) 0.4026(5) 0.0160(3) 0.030(2) Uani 1 1 d . . . . .
O6 O 0.0631(6) -0.0196(4) 0.0711(2) 0.0209(18) Uani 1 1 d . . . . .
O7 O 0.2071(6) -0.0956(4) 0.1170(2) 0.0165(16) Uani 1 1 d . . . . .
O8 O 0.2303(6) 0.0564(4) 0.1133(2) 0.0164(17) Uani 1 1 d . . . . .
O9 O 0.0995(6) 0.2766(4) 0.0522(2) 0.0192(17) Uani 1 1 d . . . . .
O10 O 0.4558(7) 0.3373(5) 0.0666(2) 0.029(2) Uani 1 1 d . . . . .
O11 O 0.2322(7) -0.1905(5) 0.0547(2) 0.027(2) Uani 1 1 d . . . . .
O12 O 0.4272(8) 0.4387(5) 0.1199(3) 0.035(2) Uani 1 1 d . . . . .
O13 O 0.1793(6) -0.0127(4) 0.1787(2) 0.0203(18) Uani 1 1 d . . . . .
O14 O 0.1300(7) 0.3229(5) -0.0264(2) 0.0238(19) Uani 1 1 d . . . . .
O15 O 0.3990(7) -0.1236(5) 0.0955(2) 0.0227(18) Uani 1 1 d . . . . .
O16 O 0.0164(6) 0.0758(5) 0.1296(2) 0.0210(18) Uani 1 1 d . . . . .
O17 O 0.4366(6) 0.0321(4) 0.0859(2) 0.0229(19) Uani 1 1 d . . . . .
O18 O 0.0350(7) 0.2250(5) 0.1206(2) 0.025(2) Uani 1 1 d . . . . .
O19 O 0.1113(7) 0.4262(4) 0.0372(2) 0.0216(18) Uani 1 1 d . . . . .
O20 O 0.3765(6) -0.0316(5) 0.1575(2) 0.0207(18) Uani 1 1 d . . . . .
O21 O 0.0677(8) 0.3815(5) 0.1069(2) 0.030(2) Uani 1 1 d . . . . .
O22 O 0.5337(7) -0.0206(5) 0.2286(3) 0.031(2) Uani 1 1 d . . . . .
O23 O 0.2305(8) 0.4606(5) 0.1413(2) 0.032(2) Uani 1 1 d . . . . .
O24 O 0.2182(7) 0.3094(5) 0.1583(2) 0.026(2) Uani 1 1 d . . . . .
O25 O 0.4798(9) 0.4974(6) 0.0476(3) 0.044(3) Uani 1 1 d . . . . .
O26 O 0.4535(7) 0.1789(5) 0.0766(2) 0.0235(19) Uani 1 1 d . . . . .
O27 O 0.0109(7) -0.0836(5) 0.1375(2) 0.028(2) Uani 1 1 d . . . . .
O28 O 0.0777(9) 0.5442(5) 0.0910(3) 0.039(3) Uani 1 1 d . . . . .
O29 O 0.3476(8) 0.0581(5) 0.2186(2) 0.028(2) Uani 1 1 d . . . . .
O30 O 0.2489(7) 0.2033(4) 0.1045(2) 0.0212(18) Uani 1 1 d . . . . .
O31 O 0.3502(7) -0.1855(4) 0.1599(2) 0.025(2) Uani 1 1 d . . . . .
O32 O 0.2889(6) 0.2551(5) 0.0325(2) 0.0204(18) Uani 1 1 d . . . . .
O33 O 0.2765(7) 0.5064(5) 0.0710(2) 0.031(2) Uani 1 1 d . . . . .
O34 O 0.1554(7) -0.1649(5) 0.1818(2) 0.0244(19) Uani 1 1 d . . . . .
O35 O 0.5903(9) 0.4804(7) 0.2051(3) 0.049(3) Uani 1 1 d . . . . .
O36 O 0.5623(6) 0.0378(5) 0.1547(3) 0.0236(19) Uani 1 1 d . . . . .
O37 O 0.5685(9) 0.2947(6) 0.2084(3) 0.045(3) Uani 1 1 d . . . . .
O38 O 0.2203(8) 0.1664(5) 0.2448(2) 0.032(2) Uani 1 1 d . . . . .
O39 O 0.4133(7) 0.2880(5) 0.1375(2) 0.027(2) Uani 1 1 d . . . . .
O40 O 0.1810(7) -0.2548(4) 0.1201(2) 0.028(2) Uani 1 1 d . . . . .
O41 O 0.2621(7) 0.3521(4) 0.0886(2) 0.0237(19) Uani 1 1 d . . . . .
O42 O 0.5791(6) 0.1925(5) 0.1447(3) 0.028(2) Uani 1 1 d . . . . .
O43 O 0.3680(8) 0.2374(5) 0.2068(2) 0.032(2) Uani 1 1 d . . . . .
O44 O 0.5297(6) 0.1359(5) 0.2124(2) 0.0219(18) Uiso 1 1 d . . . . .
O45 O 0.0381(7) -0.1702(5) 0.0760(3) 0.026(2) Uani 1 1 d . . . . .
O46 O 0.3404(6) -0.1090(4) 0.2288(2) 0.0191(17) Uani 1 1 d . . . . .
O47 O 0.3858(8) -0.2890(5) 0.0980(3) 0.036(2) Uani 1 1 d . . . . .
O48 O 0.6425(9) 0.0933(6) 0.0895(3) 0.049(3) Uani 1 1 d . . . . .
O49 O 0.0693(7) 0.2439(5) 0.1982(2) 0.028(2) Uani 1 1 d . . . . .
O50 O 0.2004(7) 0.1480(4) 0.1690(2) 0.0210(18) Uani 1 1 d . . . . .
O51 O 0.1936(8) 0.0116(5) 0.2619(2) 0.029(2) Uani 1 1 d . . . . .
O52 O 0.4545(10) 0.3339(7) 0.2667(5) 0.079(4) Uani 1 1 d . U . . .
O53 O 0.2316(9) 0.3248(5) 0.2438(3) 0.043(3) Uani 1 1 d . . . . .
O54 O -0.0259(8) -0.2456(6) 0.1429(3) 0.046(3) Uani 1 1 d . . . . .
O55 O -0.1202(8) 0.1708(7) 0.1674(3) 0.046(3) Uani 1 1 d . . . . .
O56 O -0.0954(7) 0.4386(5) 0.0071(3) 0.028(2) Uani 1 1 d . . . . .
O57 O -0.1115(8) 0.2616(5) 0.0272(3) 0.032(2) Uani 1 1 d . . . . .
O58 O 0.6919(7) 0.4849(5) 0.0424(3) 0.028(2) Uani 1 1 d . . . . .
O59 O 0.8511(7) 0.3832(5) 0.0975(3) 0.030(2) Uani 1 1 d . . . . .
O60 O 0.8803(9) 0.5898(6) 0.0930(3) 0.048(3) Uani 1 1 d . . . . .
O61 O 0.6395(11) 0.4176(9) 0.1347(3) 0.066(4) Uani 1 1 d . . . . .
O62 O 0.8723(12) 0.5063(9) 0.1691(3) 0.070(4) Uani 1 1 d . . . . .
O63 O 0.7801(18) 0.6776(14) 0.1795(5) 0.126(8) Uani 1 1 d . . . . .
O64 O -0.2894(8) 0.3628(5) -0.0336(3) 0.037(2) Uani 1 1 d . . . . .
O65 O -0.3554(10) 0.2955(7) 0.0465(5) 0.075(5) Uani 1 1 d . . . . .
O66 O -0.1401(6) -0.1145(4) -0.0322(2) 0.0138(15) Uiso 1 1 d . U . . .
O67 O 0.6713(6) 0.0554(5) 0.2875(2) 0.0223(18) Uiso 1 1 d . U . . .
O68 O 0.4366(7) 0.1529(5) 0.2818(3) 0.028(2) Uiso 1 1 d . U . . .
O69 O 0.0514(7) 0.0897(5) 0.2077(2) 0.028(2) Uani 1 1 d . . . . .
O70 O 0.2838(8) 0.0204(9) -0.0665(3) 0.064(4) Uani 1 1 d . . . . .
O71 O -0.0555(10) -0.3711(5) 0.1602(3) 0.055(4) Uani 1 1 d . . . . .
O72 O 0.8570(18) 0.0660(15) 0.0607(7) 0.142(8) Uani 1 1 d . U . . .
O73 O 0.4423(12) -0.4115(6) 0.1471(4) 0.067(4) Uani 1 1 d . . . . .
O74 O 0.5197(13) 0.6366(7) 0.0222(5) 0.085(5) Uani 1 1 d . . . . .
O75 O 0.1497(16) -0.3786(7) 0.1626(4) 0.090(6) Uani 1 1 d . . . . .
O76 O 0.3540(13) -0.2920(8) 0.2166(4) 0.078(4) Uani 1 1 d . U . . .
O77 O 0.8277(10) 0.1551(8) 0.0809(4) 0.059(3) Uiso 1 1 d . U . . .
O78 O 0.663(2) 0.5777(17) 0.1334(13) 0.235(19) Uani 1 1 d . . . . .
O79 O 0.7938(11) 0.2014(8) 0.0893(4) 0.063(3) Uiso 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Nb1 O1 2.488(9) . ?
Nb1 O17 2.065(8) . ?
Nb1 O26 2.064(8) . ?
Nb1 O36 1.919(8) . ?
Nb1 O42 1.924(9) . ?
Nb1 O48 1.691(14) . ?
Nb2 O10 1.873(8) . ?
Nb2 O26 1.827(9) . ?
Nb2 O30 2.188(8) . ?
Nb2 O32 1.894(8) . ?
Nb2 O39 2.073(9) . ?
Nb2 O41 2.242(9) . ?
Nb3 O5 1.947(9) . ?
Nb3 O9 2.033(8) . ?
Nb3 O14 1.769(8) . ?
Nb3 O19 1.974(9) . ?
Nb3 O32 2.030(8) . ?
Nb3 O41 2.467(8) . ?
Nb4 O7 2.337(7) . ?
Nb4 O13 2.102(9) . ?
Nb4 O20 2.087(8) . ?
Nb4 O31 1.940(9) . ?
Nb4 O34 1.953(8) . ?
Nb4 O46 1.770(7) . ?
Nb5 O6 1.905(8) . ?
Nb5 O7 2.230(8) . ?
Nb5 O8 2.181(8) . ?
Nb5 O13 2.075(8) . ?
Nb5 O16 1.815(9) . ?
Nb5 O27 1.881(9) . ?
Nb6 O2 1.891(8) . ?
Nb6 O7 2.239(8) . ?
Nb6 O8 2.206(8) . ?
Nb6 O15 1.879(9) . ?
Nb6 O17 1.827(8) . ?
Nb6 O20 2.081(8) . ?
Nb7 O13 2.094(8) . ?
Nb7 O29 1.927(10) . ?
Nb7 O38 1.967(9) . ?
Nb7 O50 2.383(8) . ?
Nb7 O51 1.743(8) . ?
Nb7 O69 2.013(9) . ?
Nb8 O1 2.358(8) . ?
Nb8 O20 2.101(8) . ?
Nb8 O22 1.774(9) . ?
Nb8 O29 1.925(10) . ?
Nb8 O36 1.997(9) . ?
Nb8 O44 1.962(8) . ?
Nb9 O5 2.006(9) . ?
Nb9 O10 2.048(10) . ?
Nb9 O12 1.980(9) . ?
Nb9 O25 1.733(10) . ?
Nb9 O33 1.940(10) . ?
Nb9 O41 2.544(9) . ?
Nb10 O9 1.914(8) . ?
Nb10 O18 1.799(9) . ?
Nb10 O21 1.883(9) . ?
Nb10 O24 2.071(8) . ?
Nb10 O30 2.183(9) . ?
Nb10 O41 2.249(9) . ?
Nb11 O16 2.072(9) . ?
Nb11 O18 2.090(9) . ?
Nb11 O49 1.904(9) . ?
Nb11 O50 2.447(9) . ?
Nb11 O55 1.760(11) . ?
Nb11 O69 1.921(8) . ?
Nb12 K1 4.119(3) 3_565 ?
Nb12 O19 1.989(8) . ?
Nb12 O21 2.042(10) . ?
Nb12 O23 1.977(9) . ?
Nb12 O28 1.716(10) . ?
Nb12 O33 1.968(10) . ?
Nb12 O41 2.514(8) . ?
Nb13 O1 2.377(8) . ?
Nb13 O37 1.787(9) . ?
Nb13 O39 2.091(9) . ?
Nb13 O42 1.998(10) . ?
Nb13 O43 1.920(11) . ?
Nb13 O44 1.962(8) . ?
Nb14 O3 1.768(8) . ?
Nb14 O12 1.979(10) . ?
Nb14 O23 1.951(10) . ?
Nb14 O24 2.094(9) . ?
Nb14 O39 2.080(10) . ?
Nb14 O41 2.323(8) . ?
Nb15 K1 3.833(3) 3 ?
Nb15 O7 2.527(8) . ?
Nb15 O27 2.048(9) . ?
Nb15 O34 1.982(8) . ?
Nb15 O40 1.969(10) . ?
Nb15 O45 1.990(9) . ?
Nb15 O54 1.748(10) . ?
Nb16 K1 3.880(3) 3 ?
Nb16 O2 2.025(8) . ?
Nb16 O4 1.766(8) . ?
Nb16 O6 2.022(9) . ?
Nb16 O7 2.437(7) . ?
Nb16 O11 1.976(9) . ?
Nb16 O45 1.943(9) . ?
Nb17 K1 3.844(3) 3 ?
Nb17 O7 2.544(8) . ?
Nb17 O11 1.983(8) . ?
Nb17 O15 2.047(8) . ?
Nb17 O31 1.973(8) . ?
Nb17 O40 1.970(9) . ?
Nb17 O47 1.763(10) . ?
Nb18 O24 2.112(8) . ?
Nb18 O38 1.971(9) . ?
Nb18 O43 1.924(11) . ?
Nb18 O49 2.017(10) . ?
Nb18 O50 2.376(8) . ?
Nb18 O53 1.762(9) . ?
Co1 O3 2.025(9) . ?
Co1 O22 2.130(9) 2_655 ?
Co1 O35 2.206(11) . ?
Co1 O37 2.208(12) . ?
Co1 O46 2.034(8) 2_655 ?
Co1 O52 1.804(19) . ?
Si1 O1 1.631(8) . ?
Si1 O8 1.644(8) . ?
Si1 O30 1.650(8) . ?
Si1 O50 1.625(9) . ?
K1 O11 3.034(9) 3 ?
K1 O14 2.834(9) . ?
K1 O28 2.840(10) 3_565 ?
K1 O40 2.900(9) 3 ?
K1 O45 2.993(9) 3 ?
K1 O56 2.916(10) . ?
K1 O57 2.985(10) . ?
K1 O64 2.885(12) . ?
Na1 Na2 3.609(8) 1_455 ?
Na1 O56 2.321(10) . ?
Na1 O57 2.457(11) . ?
Na1 O58 2.407(11) 1_455 ?
Na1 O59 2.420(11) 1_455 ?
Na1 O64 2.345(10) . ?
Na1 O65 2.331(13) . ?
Na2 O58 2.406(11) . ?
Na2 O59 2.442(11) . ?
Na2 O60 2.389(13) . ?
Na2 O61 2.434(15) . ?
Na2 O62 2.419(14) . ?
Na2 O78 2.19(3) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O17 Nb1 O1 80.3(3) . . ?
O26 Nb1 O1 79.9(3) . . ?
O26 Nb1 O17 81.0(3) . . ?
O36 Nb1 O1 75.4(3) . . ?
O36 Nb1 O17 87.1(3) . . ?
O36 Nb1 O26 154.1(3) . . ?
O36 Nb1 O42 94.7(4) . . ?
O42 Nb1 O1 74.9(3) . . ?
O42 Nb1 O17 153.8(4) . . ?
O42 Nb1 O26 86.4(3) . . ?
O48 Nb1 O1 179.1(4) . . ?
O48 Nb1 O17 100.5(4) . . ?
O48 Nb1 O26 100.5(4) . . ?
O48 Nb1 O36 104.3(4) . . ?
O48 Nb1 O42 104.3(5) . . ?
O10 Nb2 O30 160.1(4) . . ?
O10 Nb2 O32 94.7(4) . . ?
O10 Nb2 O39 90.0(4) . . ?
O10 Nb2 O41 84.1(4) . . ?
O26 Nb2 O10 102.2(4) . . ?
O26 Nb2 O30 96.9(3) . . ?
O26 Nb2 O32 99.1(4) . . ?
O26 Nb2 O39 101.4(4) . . ?
O26 Nb2 O41 173.7(3) . . ?
O30 Nb2 O41 76.8(3) . . ?
O32 Nb2 O30 87.6(3) . . ?
O32 Nb2 O39 157.5(4) . . ?
O32 Nb2 O41 81.4(3) . . ?
O39 Nb2 O30 80.7(3) . . ?
O39 Nb2 O41 77.3(3) . . ?
O5 Nb3 O9 152.5(3) . . ?
O5 Nb3 O19 89.8(4) . . ?
O5 Nb3 O32 86.9(4) . . ?
O5 Nb3 O41 79.7(3) . . ?
O9 Nb3 O41 72.9(3) . . ?
O14 Nb3 O5 103.8(4) . . ?
O14 Nb3 O9 103.5(4) . . ?
O14 Nb3 O19 104.5(4) . . ?
O14 Nb3 O32 103.7(4) . . ?
O14 Nb3 O41 175.5(3) . . ?
O19 Nb3 O9 87.0(3) . . ?
O19 Nb3 O32 151.5(3) . . ?
O19 Nb3 O41 78.2(3) . . ?
O32 Nb3 O9 83.1(3) . . ?
O32 Nb3 O41 73.4(3) . . ?
O13 Nb4 O7 75.3(3) . . ?
O20 Nb4 O7 75.7(3) . . ?
O20 Nb4 O13 84.2(3) . . ?
O31 Nb4 O7 80.0(3) . . ?
O31 Nb4 O13 155.2(3) . . ?
O31 Nb4 O20 88.0(4) . . ?
O31 Nb4 O34 91.6(4) . . ?
O34 Nb4 O7 80.3(3) . . ?
O34 Nb4 O13 86.0(3) . . ?
O34 Nb4 O20 155.7(3) . . ?
O46 Nb4 O7 176.5(3) . . ?
O46 Nb4 O13 105.6(3) . . ?
O46 Nb4 O20 100.9(3) . . ?
O46 Nb4 O31 99.0(3) . . ?
O46 Nb4 O34 103.1(4) . . ?
O6 Nb5 O7 80.6(3) . . ?
O6 Nb5 O8 87.2(3) . . ?
O6 Nb5 O13 157.9(4) . . ?
O8 Nb5 O7 77.6(3) . . ?
O13 Nb5 O7 78.2(3) . . ?
O13 Nb5 O8 82.1(3) . . ?
O16 Nb5 O6 99.0(4) . . ?
O16 Nb5 O7 172.7(3) . . ?
O16 Nb5 O8 95.1(3) . . ?
O16 Nb5 O13 101.2(4) . . ?
O16 Nb5 O27 102.9(4) . . ?
O27 Nb5 O6 95.0(4) . . ?
O27 Nb5 O7 84.4(3) . . ?
O27 Nb5 O8 161.2(3) . . ?
O27 Nb5 O13 89.2(3) . . ?
O2 Nb6 O7 80.4(3) . . ?
O2 Nb6 O8 86.9(3) . . ?
O2 Nb6 O20 157.3(3) . . ?
O8 Nb6 O7 76.9(3) . . ?
O15 Nb6 O2 95.1(4) . . ?
O15 Nb6 O7 84.1(3) . . ?
O15 Nb6 O8 160.3(3) . . ?
O15 Nb6 O20 90.0(3) . . ?
O17 Nb6 O2 100.9(4) . . ?
O17 Nb6 O7 173.5(4) . . ?
O17 Nb6 O8 96.9(3) . . ?
O17 Nb6 O15 102.0(4) . . ?
O17 Nb6 O20 99.7(3) . . ?
O20 Nb6 O7 78.1(3) . . ?
O20 Nb6 O8 81.1(3) . . ?
O13 Nb7 O50 81.6(3) . . ?
O29 Nb7 O13 86.4(3) . . ?
O29 Nb7 O38 92.3(4) . . ?
O29 Nb7 O50 84.2(3) . . ?
O29 Nb7 O69 160.2(3) . . ?
O38 Nb7 O13 157.1(3) . . ?
O38 Nb7 O50 75.5(3) . . ?
O38 Nb7 O69 88.4(4) . . ?
O51 Nb7 O13 100.6(4) . . ?
O51 Nb7 O29 100.7(4) . . ?
O51 Nb7 O38 102.0(4) . . ?
O51 Nb7 O50 174.6(4) . . ?
O51 Nb7 O69 98.4(4) . . ?
O69 Nb7 O13 85.3(4) . . ?
O69 Nb7 O50 76.8(3) . . ?
O20 Nb8 O1 81.2(3) . . ?
O22 Nb8 O1 175.4(3) . . ?
O22 Nb8 O20 102.4(4) . . ?
O22 Nb8 O29 98.3(4) . . ?
O22 Nb8 O36 100.2(4) . . ?
O22 Nb8 O44 100.8(4) . . ?
O29 Nb8 O1 84.7(3) . . ?
O29 Nb8 O20 86.9(3) . . ?
O29 Nb8 O36 160.9(3) . . ?
O29 Nb8 O44 92.3(4) . . ?
O36 Nb8 O1 77.2(3) . . ?
O36 Nb8 O20 84.2(3) . . ?
O44 Nb8 O1 75.5(3) . . ?
O44 Nb8 O20 156.7(3) . . ?
O44 Nb8 O36 89.3(3) . . ?
O5 Nb9 O10 85.2(4) . . ?
O5 Nb9 O41 76.8(3) . . ?
O10 Nb9 O41 73.3(3) . . ?
O12 Nb9 O5 150.9(4) . . ?
O12 Nb9 O10 83.9(4) . . ?
O12 Nb9 O41 74.3(3) . . ?
O25 Nb9 O5 104.2(4) . . ?
O25 Nb9 O10 104.3(5) . . ?
O25 Nb9 O12 104.6(4) . . ?
O25 Nb9 O33 104.2(5) . . ?
O25 Nb9 O41 177.4(4) . . ?
O33 Nb9 O5 88.8(4) . . ?
O33 Nb9 O10 151.5(4) . . ?
O33 Nb9 O12 88.0(4) . . ?
O33 Nb9 O41 78.2(3) . . ?
O9 Nb10 O24 157.2(4) . . ?
O9 Nb10 O30 86.9(3) . . ?
O9 Nb10 O41 80.3(3) . . ?
O18 Nb10 O9 99.5(3) . . ?
O18 Nb10 O21 104.2(4) . . ?
O18 Nb10 O24 101.0(4) . . ?
O18 Nb10 O30 95.6(4) . . ?
O18 Nb10 O41 172.4(4) . . ?
O21 Nb10 O9 94.3(4) . . ?
O21 Nb10 O24 90.3(4) . . ?
O21 Nb10 O30 159.7(4) . . ?
O21 Nb10 O41 83.5(4) . . ?
O24 Nb10 O30 81.3(3) . . ?
O24 Nb10 O41 78.1(3) . . ?
O30 Nb10 O41 76.7(3) . . ?
O16 Nb11 O18 81.8(3) . . ?
O16 Nb11 O50 79.8(3) . . ?
O18 Nb11 O50 79.6(3) . . ?
O49 Nb11 O16 155.6(4) . . ?
O49 Nb11 O18 86.8(3) . . ?
O49 Nb11 O50 77.0(3) . . ?
O49 Nb11 O69 94.8(4) . . ?
O55 Nb11 O16 99.5(5) . . ?
O55 Nb11 O18 100.3(4) . . ?
O55 Nb11 O49 103.7(5) . . ?
O55 Nb11 O50 179.3(5) . . ?
O55 Nb11 O69 103.1(5) . . ?
O69 Nb11 O16 87.1(4) . . ?
O69 Nb11 O18 155.5(4) . . ?
O69 Nb11 O50 76.9(3) . . ?
O19 Nb12 K1 90.1(2) . 3_565 ?
O19 Nb12 O21 85.4(3) . . ?
O19 Nb12 O41 76.8(3) . . ?
O21 Nb12 K1 134.7(3) . 3_565 ?
O21 Nb12 O41 73.9(3) . . ?
O23 Nb12 K1 115.2(3) . 3_565 ?
O23 Nb12 O19 151.9(4) . . ?
O23 Nb12 O21 84.6(4) . . ?
O23 Nb12 O41 75.3(3) . . ?
O28 Nb12 K1 33.1(4) . 3_565 ?
O28 Nb12 O19 104.4(4) . . ?
O28 Nb12 O21 105.4(5) . . ?
O28 Nb12 O23 103.5(4) . . ?
O28 Nb12 O33 102.3(5) . . ?
O28 Nb12 O41 178.6(4) . . ?
O33 Nb12 K1 71.9(3) . 3_565 ?
O33 Nb12 O19 87.4(4) . . ?
O33 Nb12 O21 152.3(4) . . ?
O33 Nb12 O23 89.3(4) . . ?
O33 Nb12 O41 78.5(3) . . ?
O41 Nb12 K1 148.1(2) . 3_565 ?
O37 Nb13 O1 176.3(5) . . ?
O37 Nb13 O39 101.2(4) . . ?
O37 Nb13 O42 101.5(5) . . ?
O37 Nb13 O43 98.6(5) . . ?
O37 Nb13 O44 102.0(4) . . ?
O39 Nb13 O1 81.6(3) . . ?
O42 Nb13 O1 76.3(3) . . ?
O42 Nb13 O39 84.7(4) . . ?
O43 Nb13 O1 83.8(3) . . ?
O43 Nb13 O39 86.9(4) . . ?
O43 Nb13 O42 159.3(3) . . ?
O43 Nb13 O44 91.6(4) . . ?
O44 Nb13 O1 75.1(3) . . ?
O44 Nb13 O39 156.7(3) . . ?
O44 Nb13 O42 88.7(4) . . ?
O3 Nb14 O12 100.7(4) . . ?
O3 Nb14 O23 102.4(4) . . ?
O3 Nb14 O24 103.5(4) . . ?
O3 Nb14 O39 101.8(4) . . ?
O3 Nb14 O41 177.1(3) . . ?
O12 Nb14 O24 155.4(3) . . ?
O12 Nb14 O39 87.2(4) . . ?
O12 Nb14 O41 79.7(3) . . ?
O23 Nb14 O12 91.5(4) . . ?
O23 Nb14 O24 87.6(4) . . ?
O23 Nb14 O39 155.6(3) . . ?
O23 Nb14 O41 80.5(3) . . ?
O24 Nb14 O41 76.0(3) . . ?
O39 Nb14 O24 83.7(3) . . ?
O39 Nb14 O41 75.3(3) . . ?
O7 Nb15 K1 98.23(19) . 3 ?
O27 Nb15 K1 135.6(2) . 3 ?
O27 Nb15 O7 73.8(3) . . ?
O34 Nb15 K1 136.7(3) . 3 ?
O34 Nb15 O7 75.1(3) . . ?
O34 Nb15 O27 84.5(4) . . ?
O34 Nb15 O45 151.0(3) . . ?
O40 Nb15 K1 47.7(2) . 3 ?
O40 Nb15 O7 79.1(3) . . ?
O40 Nb15 O27 152.9(4) . . ?
O40 Nb15 O34 89.5(4) . . ?
O40 Nb15 O45 87.0(4) . . ?
O45 Nb15 K1 50.6(3) . 3 ?
O45 Nb15 O7 75.9(3) . . ?
O45 Nb15 O27 85.6(4) . . ?
O54 Nb15 K1 84.5(4) . 3 ?
O54 Nb15 O7 176.5(5) . . ?
O54 Nb15 O27 102.7(5) . . ?
O54 Nb15 O34 104.5(4) . . ?
O54 Nb15 O40 104.4(5) . . ?
O54 Nb15 O45 104.3(4) . . ?
O2 Nb16 K1 137.4(2) . 3 ?
O2 Nb16 O7 73.2(3) . . ?
O4 Nb16 K1 84.5(3) . 3 ?
O4 Nb16 O2 104.8(4) . . ?
O4 Nb16 O6 104.0(4) . . ?
O4 Nb16 O7 176.8(3) . . ?
O4 Nb16 O11 102.8(4) . . ?
O4 Nb16 O45 103.0(4) . . ?
O6 Nb16 K1 136.4(2) . 3 ?
O6 Nb16 O2 82.4(3) . . ?
O6 Nb16 O7 73.4(3) . . ?
O7 Nb16 K1 98.69(19) . 3 ?
O11 Nb16 K1 50.5(3) . 3 ?
O11 Nb16 O2 87.1(3) . . ?
O11 Nb16 O6 152.9(3) . . ?
O11 Nb16 O7 79.7(3) . . ?
O45 Nb16 K1 49.1(3) . 3 ?
O45 Nb16 O2 152.0(3) . . ?
O45 Nb16 O6 87.6(4) . . ?
O45 Nb16 O7 78.9(3) . . ?
O45 Nb16 O11 90.2(4) . . ?
O7 Nb17 K1 97.64(17) . 3 ?
O11 Nb17 K1 51.4(3) . 3 ?
O11 Nb17 O7 76.9(3) . . ?
O11 Nb17 O15 85.0(3) . . ?
O15 Nb17 K1 136.2(2) . 3 ?
O15 Nb17 O7 73.4(3) . . ?
O31 Nb17 K1 135.6(3) . 3 ?
O31 Nb17 O7 74.3(3) . . ?
O31 Nb17 O11 151.1(3) . . ?
O31 Nb17 O15 84.3(3) . . ?
O40 Nb17 K1 47.4(3) . 3 ?
O40 Nb17 O7 78.7(3) . . ?
O40 Nb17 O11 88.5(4) . . ?
O40 Nb17 O15 152.1(4) . . ?
O40 Nb17 O31 88.5(4) . . ?
O47 Nb17 K1 85.3(3) . 3 ?
O47 Nb17 O7 176.5(4) . . ?
O47 Nb17 O11 103.5(4) . . ?
O47 Nb17 O15 103.1(4) . . ?
O47 Nb17 O31 105.0(4) . . ?
O47 Nb17 O40 104.8(4) . . ?
O24 Nb18 O50 82.0(3) . . ?
O38 Nb18 O24 157.6(3) . . ?
O38 Nb18 O49 87.9(4) . . ?
O38 Nb18 O50 75.6(3) . . ?
O43 Nb18 O24 85.5(4) . . ?
O43 Nb18 O38 92.7(4) . . ?
O43 Nb18 O49 159.8(3) . . ?
O43 Nb18 O50 83.9(3) . . ?
O49 Nb18 O24 86.3(4) . . ?
O49 Nb18 O50 76.7(3) . . ?
O53 Nb18 O24 102.3(4) . . ?
O53 Nb18 O38 100.0(4) . . ?
O53 Nb18 O43 100.7(5) . . ?
O53 Nb18 O49 99.1(5) . . ?
O53 Nb18 O50 173.9(4) . . ?
O3 Co1 O22 92.6(4) . 2_655 ?
O3 Co1 O35 85.6(4) . . ?
O3 Co1 O37 89.3(4) . . ?
O3 Co1 O46 170.1(4) . 2_655 ?
O22 Co1 O35 89.0(4) 2_655 . ?
O22 Co1 O37 171.5(4) 2_655 . ?
O35 Co1 O37 99.4(4) . . ?
O46 Co1 O22 91.8(3) 2_655 2_655 ?
O46 Co1 O35 85.6(4) 2_655 . ?
O46 Co1 O37 87.7(4) 2_655 . ?
O52 Co1 O3 93.2(5) . . ?
O52 Co1 O22 83.6(5) . 2_655 ?
O52 Co1 O35 172.4(5) . . ?
O52 Co1 O37 88.1(5) . . ?
O52 Co1 O46 96.1(5) . 2_655 ?
O1 Si1 O8 108.6(4) . . ?
O1 Si1 O30 108.2(4) . . ?
O8 Si1 O30 109.0(4) . . ?
O50 Si1 O1 114.5(4) . . ?
O50 Si1 O8 108.1(4) . . ?
O50 Si1 O30 108.3(5) . . ?
Nb15 K1 Nb12 110.87(7) 3 3_565 ?
Nb15 K1 Nb16 52.07(4) 3 3 ?
Nb15 K1 Nb17 52.32(5) 3 3 ?
Nb16 K1 Nb12 152.72(8) 3 3_565 ?
Nb17 K1 Nb12 101.08(7) 3 3_565 ?
Nb17 K1 Nb16 51.94(4) 3 3 ?
O11 K1 Nb12 127.09(19) 3 3_565 ?
O11 K1 Nb15 63.50(18) 3 3 ?
O11 K1 Nb16 30.16(18) 3 3 ?
O11 K1 Nb17 30.74(16) 3 3 ?
O14 K1 Nb12 104.29(19) . 3_565 ?
O14 K1 Nb15 93.8(2) . 3 ?
O14 K1 Nb16 98.51(19) . 3 ?
O14 K1 Nb17 143.5(2) . 3 ?
O14 K1 O11 128.0(3) . 3 ?
O14 K1 O28 91.9(3) . 3_565 ?
O14 K1 O40 122.5(3) . 3 ?
O14 K1 O45 81.3(2) . 3 ?
O14 K1 O56 86.3(3) . . ?
O14 K1 O57 88.6(3) . . ?
O14 K1 O64 148.6(3) . . ?
O28 K1 Nb12 19.3(2) 3_565 3_565 ?
O28 K1 Nb15 97.6(2) 3_565 3 ?
O28 K1 Nb16 148.3(2) 3_565 3 ?
O28 K1 Nb17 104.5(2) 3_565 3 ?
O28 K1 O11 134.7(3) 3_565 3 ?
O28 K1 O40 87.1(3) 3_565 3 ?
O28 K1 O45 125.9(3) 3_565 3 ?
O28 K1 O56 75.7(3) 3_565 . ?
O28 K1 O57 143.2(3) 3_565 . ?
O28 K1 O64 89.4(3) 3_565 . ?
O40 K1 Nb12 92.66(18) 3 3_565 ?
O40 K1 Nb15 30.1(2) 3 3 ?
O40 K1 Nb16 62.10(17) 3 3 ?
O40 K1 Nb17 30.02(19) 3 3 ?
O40 K1 O11 55.3(2) 3 3 ?
O40 K1 O45 55.1(2) 3 3 ?
O40 K1 O56 147.3(3) 3 . ?
O40 K1 O57 123.0(3) 3 . ?
O45 K1 Nb12 141.42(19) 3 3_565 ?
O45 K1 Nb15 30.89(17) 3 3 ?
O45 K1 Nb16 29.40(18) 3 3 ?
O45 K1 Nb17 62.66(16) 3 3 ?
O45 K1 O11 54.8(3) 3 3 ?
O56 K1 Nb12 62.74(18) . 3_565 ?
O56 K1 Nb15 173.3(2) . 3 ?
O56 K1 Nb16 134.5(2) . 3 ?
O56 K1 Nb17 129.0(2) . 3 ?
O56 K1 O11 121.4(3) . 3 ?
O56 K1 O45 155.1(3) . 3 ?
O56 K1 O57 67.6(2) . . ?
O57 K1 Nb12 127.3(2) . 3_565 ?
O57 K1 Nb15 119.04(19) . 3 ?
O57 K1 Nb16 67.31(18) . 3 ?
O57 K1 Nb17 96.48(19) . 3 ?
O57 K1 O11 67.8(2) . 3 ?
O57 K1 O45 90.5(3) . 3 ?
O64 K1 Nb12 71.1(2) . 3_565 ?
O64 K1 Nb15 117.13(19) . 3 ?
O64 K1 Nb16 96.7(2) . 3 ?
O64 K1 Nb17 65.38(18) . 3 ?
O64 K1 O11 67.9(3) . 3 ?
O64 K1 O40 89.0(3) . 3 ?
O64 K1 O45 122.4(3) . 3 ?
O64 K1 O56 63.6(3) . . ?
O64 K1 O57 72.2(3) . . ?
O56 Na1 Na2 93.8(3) . 1_455 ?
O56 Na1 O57 86.8(4) . . ?
O56 Na1 O58 89.0(3) . 1_455 ?
O56 Na1 O59 95.9(4) . 1_455 ?
O56 Na1 O64 81.9(4) . . ?
O56 Na1 O65 171.6(5) . . ?
O57 Na1 Na2 130.8(3) . 1_455 ?
O58 Na1 Na2 41.4(2) 1_455 1_455 ?
O58 Na1 O57 170.8(4) 1_455 . ?
O58 Na1 O59 83.7(3) 1_455 1_455 ?
O59 Na1 Na2 42.3(2) 1_455 1_455 ?
O59 Na1 O57 88.6(3) 1_455 . ?
O64 Na1 Na2 136.7(3) . 1_455 ?
O64 Na1 O57 92.2(4) . . ?
O64 Na1 O58 95.3(4) . 1_455 ?
O64 Na1 O59 177.6(4) . 1_455 ?
O65 Na1 Na2 93.9(4) . 1_455 ?
O65 Na1 O57 90.8(5) . . ?
O65 Na1 O58 94.5(5) . 1_455 ?
O65 Na1 O59 92.1(5) . 1_455 ?
O65 Na1 O64 90.2(5) . . ?
O58 Na2 Na1 41.4(3) . 1_655 ?
O58 Na2 O59 83.3(4) . . ?
O58 Na2 O61 97.7(4) . . ?
O58 Na2 O62 165.3(5) . . ?
O59 Na2 Na1 41.8(2) . 1_655 ?
O60 Na2 Na1 98.9(3) . 1_655 ?
O60 Na2 O58 90.7(4) . . ?
O60 Na2 O59 101.8(4) . . ?
O60 Na2 O61 169.9(5) . . ?
O60 Na2 O62 80.4(5) . . ?
O61 Na2 Na1 91.2(4) . 1_655 ?
O61 Na2 O59 84.9(5) . . ?
O62 Na2 Na1 128.3(4) . 1_655 ?
O62 Na2 O59 87.2(5) . . ?
O62 Na2 O61 92.5(5) . . ?
O78 Na2 Na1 145.4(10) . 1_655 ?
O78 Na2 O58 107.1(11) . . ?
O78 Na2 O59 160.6(12) . . ?
O78 Na2 O60 94.5(11) . . ?
O78 Na2 O61 77.6(11) . . ?
O78 Na2 O62 85.3(11) . . ?
Nb8 O1 Nb1 88.1(3) . . ?
Nb8 O1 Nb13 90.8(3) . . ?
Nb13 O1 Nb1 88.5(3) . . ?
Si1 O1 Nb1 131.5(4) . . ?
Si1 O1 Nb8 123.4(4) . . ?
Si1 O1 Nb13 122.6(5) . . ?
Nb6 O2 Nb16 115.2(4) . . ?
Nb14 O3 Co1 149.0(6) . . ?
Nb3 O5 Nb9 118.0(5) . . ?
Nb5 O6 Nb16 114.8(4) . . ?
Nb4 O7 Nb15 87.1(3) . . ?
Nb4 O7 Nb16 170.2(4) . . ?
Nb4 O7 Nb17 86.9(2) . . ?
Nb5 O7 Nb4 96.4(3) . . ?
Nb5 O7 Nb6 101.1(3) . . ?
Nb5 O7 Nb15 87.5(3) . . ?
Nb5 O7 Nb16 90.2(3) . . ?
Nb5 O7 Nb17 170.5(4) . . ?
Nb6 O7 Nb4 95.8(3) . . ?
Nb6 O7 Nb15 170.5(4) . . ?
Nb6 O7 Nb16 89.9(3) . . ?
Nb6 O7 Nb17 87.4(3) . . ?
Nb15 O7 Nb17 83.8(2) . . ?
Nb16 O7 Nb15 86.0(2) . . ?
Nb16 O7 Nb17 85.5(2) . . ?
Nb5 O8 Nb6 103.7(3) . . ?
Si1 O8 Nb5 123.9(5) . . ?
Si1 O8 Nb6 123.3(4) . . ?
Nb10 O9 Nb3 115.7(4) . . ?
Nb2 O10 Nb9 115.1(5) . . ?
Nb16 O11 Nb17 117.4(4) . . ?
Nb16 O11 K1 99.3(4) . 3 ?
Nb17 O11 K1 97.8(3) . 3 ?
Nb14 O12 Nb9 117.5(4) . . ?
Nb5 O13 Nb4 109.2(4) . . ?
Nb5 O13 Nb7 129.8(4) . . ?
Nb7 O13 Nb4 119.1(4) . . ?
Nb3 O14 K1 122.6(4) . . ?
Nb6 O15 Nb17 114.9(4) . . ?
Nb5 O16 Nb11 136.9(4) . . ?
Nb6 O17 Nb1 137.3(5) . . ?
Nb10 O18 Nb11 138.0(4) . . ?
Nb3 O19 Nb12 118.5(4) . . ?
Nb4 O20 Nb8 118.1(4) . . ?
Nb6 O20 Nb4 109.2(4) . . ?
Nb6 O20 Nb8 131.1(4) . . ?
Nb10 O21 Nb12 114.8(5) . . ?
Nb8 O22 Co1 132.0(5) . 2_645 ?
Nb14 O23 Nb12 116.5(5) . . ?
Nb10 O24 Nb14 109.1(4) . . ?
Nb10 O24 Nb18 129.2(4) . . ?
Nb14 O24 Nb18 120.0(4) . . ?
Nb2 O26 Nb1 137.0(5) . . ?
Nb5 O27 Nb15 114.0(5) . . ?
Nb12 O28 K1 127.7(6) . 3_565 ?
Nb8 O29 Nb7 156.9(5) . . ?
Nb10 O30 Nb2 104.8(3) . . ?
Si1 O30 Nb2 123.3(5) . . ?
Si1 O30 Nb10 123.8(5) . . ?
Nb4 O31 Nb17 118.4(4) . . ?
Nb2 O32 Nb3 115.0(4) . . ?
Nb9 O33 Nb12 119.6(4) . . ?
Nb4 O34 Nb15 116.9(4) . . ?
Nb1 O36 Nb8 118.9(4) . . ?
Nb13 O37 Co1 128.6(7) . . ?
Nb7 O38 Nb18 118.3(4) . . ?
Nb2 O39 Nb13 130.1(5) . . ?
Nb2 O39 Nb14 110.0(4) . . ?
Nb14 O39 Nb13 118.5(4) . . ?
Nb15 O40 Nb17 118.5(4) . . ?
Nb15 O40 K1 102.2(3) . 3 ?
Nb17 O40 K1 102.6(4) . 3 ?
Nb2 O41 Nb3 89.2(3) . . ?
Nb2 O41 Nb9 87.3(3) . . ?
Nb2 O41 Nb10 100.9(3) . . ?
Nb2 O41 Nb12 170.3(4) . . ?
Nb2 O41 Nb14 96.3(3) . . ?
Nb3 O41 Nb9 85.1(3) . . ?
Nb3 O41 Nb12 86.2(3) . . ?
Nb10 O41 Nb3 90.1(3) . . ?
Nb10 O41 Nb9 170.5(4) . . ?
Nb10 O41 Nb12 87.7(3) . . ?
Nb10 O41 Nb14 95.8(3) . . ?
Nb12 O41 Nb9 83.8(2) . . ?
Nb14 O41 Nb3 171.0(4) . . ?
Nb14 O41 Nb9 88.0(3) . . ?
Nb14 O41 Nb12 87.2(3) . . ?
Nb1 O42 Nb13 119.9(4) . . ?
Nb13 O43 Nb18 157.7(5) . . ?
Nb8 O44 Nb13 118.5(4) . . ?
Nb15 O45 K1 98.5(3) . 3 ?
Nb16 O45 Nb15 118.8(4) . . ?
Nb16 O45 K1 101.5(4) . 3 ?
Nb4 O46 Co1 144.0(5) . 2_645 ?
Nb11 O49 Nb18 117.8(4) . . ?
Nb7 O50 Nb11 88.3(3) . . ?
Nb18 O50 Nb7 90.5(2) . . ?
Nb18 O50 Nb11 88.3(3) . . ?
Si1 O50 Nb7 123.1(5) . . ?
Si1 O50 Nb11 131.7(4) . . ?
Si1 O50 Nb18 122.9(4) . . ?
Na1 O56 K1 88.4(3) . . ?
Na1 O57 K1 84.4(3) . . ?
Na2 O58 Na1 97.1(4) . 1_655 ?
Na1 O59 Na2 95.9(4) 1_655 . ?
Na1 O64 K1 88.7(3) . . ?
Nb11 O69 Nb7 117.6(4) . . ?

_olex2_submission_special_instructions 'No special instructions were received'

# SQUEEZE RESULTS (Version = 201118)
# Note: Data are Listed for all Voids in the P1 Unit Cell
# i.e. Centre of Gravity, Solvent Accessible Volume,
# Recovered number of Electrons in the Void and
# Details about the Squeezed Material
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.119 0.354 0.310 1796 -11 ' '
_platon_squeeze_void_probe_radius 1.20
_platon_squeeze_details          ?

